ADU Lecture MEC 302 1 2 Mechanics Of Materials MEC 302 MEC 302 2 ADU Tentative Lectures Schedule Topic Reading Introduction Concept of Stress, 1.1-1.7 Introduction Concept of Stress Stress and Strain—Axial Loading, Stress and Strain—Axial Loading, Torsion, Torsion Pure Bending, Analysis and Design of Beams for Bending, Shearing Stresses in Beams and Thin-Walled Members Transformations of Stress and Strain, Transformations of Stress and Strain, Deflections of Beams Deflections of Beams Columns (Buckling) , Final Exam 1.8-1.13 2.1-2.10 2.11-2.19 3.1-3.5 3.6-3.8 4.1-4.7, 5.1-5.4 6.1-6.7, 7.1-7.3 7.4-7.9 9.1-9.5 9.7 10.1-10.6 2 Lecture 2 ADU MEC 302 3 Lecture 2 ADU MEC 302 4 Lecture 2 MEC 302 5 ADU 2.2 NORMAL STRAIN UNDER AXIAL LOADING 5 Lecture 2 MEC 302 6 ADU 2.2 NORMAL STRAIN UNDER AXIAL LOADING 6 Lecture 2 MEC 302 7 ADU 2.2 NORMAL STRAIN UNDER AXIAL LOADING 7 Lecture 2 MEC 302 8 ADU 2.3 STRESS-STRAIN DIAGRAM We saw in Sec. 2.2 that the diagram representing the relation between stress and strain in a given material is an important characteristic of the material. To obtain the stress-strain diagram of a material, one usually conducts a tensile test on a specimen of the material. One type of specimen commonly used is shown in Photo 2.1. The cross-sectional area of the cylindrical central portion of the specimen has been accurately determined and two gage marks have been inscribed on that portion at a distance L0 from each other. The distance L0 is known as the gage length of the specimen. The test specimen is then placed in a testing machine (Photo 2.2),which is used to apply a centric load P. As the load P increases, the distance L between the two gage marks also increases (Photo 2.3). 8 Lecture 2 MEC 302 9 ADU 2.3 STRESS-STRAIN DIAGRAM 9 Lecture 2 MEC 302 10 ADU 2.3 STRESS-STRAIN DIAGRAM 10 Lecture 2 ADU 11 MEC 302 2.3 STRESS-STRAIN DIAGRAM It is possible, however, to distinguish some common characteristics among the stress-strain diagrams of various groups of materials and to divide materials into two broad categories on the basis of these characteristics, namely, the ductile materials and the brittle materials. Ductile materials, which comprise structural steel, as well as many alloys of other metals, are characterized by their ability to yield at normal temperatures. As the specimen is subjected to an increasing load, its length first increases linearly with the load and at a very slow rate. Thus, the initial portion of the stress-strain diagram is a straight line with a steep slope (Fig. 2.6). However, after a critical value σY of the stress has been reached, the specimen undergoes a large deformation with a relatively small increase in the applied load. This deformation is caused by slippage of the material along oblique surfaces and is due, therefore, primarily to shearing stresses. 11 Lecture 2 ADU MEC 302 12 Lecture 2 ADU 13 MEC 302 2.3 STRESS-STRAIN DIAGRAM As we can note from the stress-strain diagrams of two typical ductile materials (Fig. 2.6), the elongation of the specimen after it has started to yield can be 200 times as large as its deformation before yield. After a certain maximum value of the load has been reached, the diameter of a portion of the specimen begins to decrease, because of local instability (Photo 2.4a). This phenomenon is known as necking. After necking has begun, somewhat lower loads are sufficient to keep the specimen elongating further, until it finally ruptures (Photo 2.4b). We note that rupture occurs along a cone-shaped surface that forms an angle of approximately 45o with the original surface of the specimen. This indicates that shear is primarily responsible for the failure of ductile materials. 13 Lecture 2 ADU 14 MEC 302 2.3 STRESS-STRAIN DIAGRAM This confirms the fact that, under an axial load, shearing stresses are largest on surfaces forming an angle of 45o with the load (cf. Sec. 1.11). The stress σY at which yield is initiated is called the yield strength of the material, the stress σU corresponding to the maximum load applied to the specimen is known as the ultimate strength, and the stress σB corresponding to rupture is called the breaking strength. Brittle materials, which comprise cast iron, glass, and stone, are characterized by the fact that rupture occurs without any noticeable prior change in the rate of elongation (Fig. 2.7). Thus, for brittle materials, there is no difference between the ultimate strength and the breaking strength. Also, the strain at the time of rupture is much smaller for brittle than for ductile materials. 14 Lecture 2 ADU MEC 302 15 Lecture 2 ADU 16 MEC 302 2.3 STRESS-STRAIN DIAGRAM From Photo 2.5, we note the absence of any necking of the specimen in the case of a brittle material, and observe that rupture occurs along a surface perpendicular to the load. We conclude from this observation that normal stresses are primarily responsible for the failure of brittle materials. The stress-strain diagrams of Fig. 2.6 show that structural steel and aluminum, while both ductile, have different yield characteristics. In the case of structural steel (Fig. 2.6a), the stress remains constant over a large range of values of the strain after the onset of yield. Later the stress must be increased to keep elongating the specimen, until the maximum value σU has been reached. This is due to a property of the material known as strain-hardening. 16 Lecture 2 ADU 17 MEC 302 2.3 STRESS-STRAIN DIAGRAM The yield strength of structural steel can be determined during the tensile test by watching the load shown on the display of the testing machine. After increasing steadily, the load is observed to suddenly drop to a slightly lower value, which is maintained for a certain period while the specimen keeps elongating. In a very carefully conducted test, one may be able to distinguish between the upper yield point, which corresponds to the load reached just before yield starts, and the lower yield point, which corresponds to the load required to maintain yield. Since the upper yield point is transient, the lower yield point should be used to determine the yield strength of the material. 17 Lecture 2 MEC 302 18 ADU 2.3 STRESS-STRAIN DIAGRAM 18 Lecture 2 ADU MEC 302 19 Lecture 2 ADU A standard measure of the ductility of a material is its percent elongation, which is defined as Another measure of ductility which is sometimes used is the percent reduction in area, defined as MEC 302 20 2.3 STRESS-STRAIN DIAGRAM 20 Lecture 2 ADU 21 MEC 302 2.3 STRESS-STRAIN DIAGRAM Thus far, we have discussed only tensile tests. If a specimen made of a ductile material were loaded in compression instead of tension. The stress-strain curve obtained would be essentially the same through its initial straight-line portion and through the beginning of the portion corresponding to yield and strain-hardening. Particularly noteworthy is the fact that for a given steel, the yield strength is the same in both tension and compression. For larger values of the strain, the tension and compression stress-strain curves diverge, and it should be noted that necking cannot occur in compression. 21 Lecture 2 ADU 22 MEC 302 2.3 STRESS-STRAIN DIAGRAM For most brittle materials, one finds that the ultimate strength in compression is much larger than the ultimate strength in tension. This is due to the presence of flaws, such as microscopic cracks or cavities, which tend to weaken the material in tension, while not appreciably affecting its resistance to compressive failure. An example of brittle material with different properties in tension and compression is provided by concrete, whose stress-strain diagram is shown in Fig. 2.9. On the tension side of the diagram, we first observe a linear elastic range in which the strain is proportional to the stress. After the yield point has been reached, the strain increases faster than the stress until rupture occurs. 22 Lecture 2 ADU The behavior of the material in compression is different. First, the linear elastic range is significantly larger. Second, rupture does not occur as the stress reaches its maximum value. Instead, the stress decreases in magnitude while the strain keeps increasing until rupture occurs. Note that the modulus of elasticity, which is represented by the slope of the stress-strain curve in its linear portion, is the same in tension and compression. This is true of most brittle materials. MEC 302 23 2.3 STRESS-STRAIN DIAGRAM 23 Lecture 2 ADU MEC 302 24 Lecture 2 ADU 25 MEC 302 2.4 TRUE STRESS AND TRUE STRAIN We recall that the stress plotted in the diagrams of Figs. 2.6 and 2.7 was obtained by dividing the load P by the cross-sectional area A0 of the specimen measured before any deformation had taken place. Since the cross-sectional area of the specimen decreases as P increases, the stress plotted in our diagrams does not represent the actual stress in the specimen. The difference between the engineering stress σ = P/A0 that we have computed and the true stress σt = P/A obtained by dividing P by the cross-sectional area A of the deformed specimen becomes apparent in ductile materials after yield has started. 25 Lecture 2 MEC 302 26 ADU 2.4 TRUE STRESS AND TRUE STRAIN 26 Lecture 2 MEC 302 27 ADU 2.4 TRUE STRESS AND TRUE STRAIN 27 Lecture 2 MEC 302 28 ADU 2.5 HOOKE’S LAW; MODULUS OF ELASTICITY 28 Lecture 2 MEC 302 29 ADU 2.5 HOOKE’S LAW; MODULUS OF ELASTICITY 29 Lecture 2 ADU MEC 302 30 Lecture 2 MEC 302 ADU Anisotropic Materials Consists of Fiberreinforced Composite Materials 31 Lecture 2 ADU 32 MEC 302 2.6 ELASTIC VERSUS PLASTIC BEHAVIOR OF A MATERIAL If the strains caused in a test specimen by the application of a given load disappear when the load is removed, the material is said to behave elastically. The largest value of the stress for which the material behaves elastically is called the elastic limit of the material. If the material has a well-defined yield point as in Fig. 2.6a, the elastic limit, the proportional limit (Sec. 2.5), and the yield point are essentially equal. In other words, the material behaves elastically and linearly as long as the stress is kept below the yield point. 32 Lecture 2 MEC 302 33 ADU 2.6 ELASTIC VERSUS PLASTIC BEHAVIOR OF A MATERIAL 33 Lecture 2 MEC 302 ADU 2.6 ELASTIC VERSUS PLASTIC BEHAVIOR OF A MATERIAL 34 Lecture 2 ADU 35 MEC 302 2.6 ELASTIC VERSUS PLASTIC BEHAVIOR OF A MATERIAL When a material does not possess a well-defined yield point, the elastic limit cannot be determined with precision. However, assuming the elastic limit equal to the yield strength as defined by the offset method (Sec. 2.3) results in only a small error. Indeed, referring to Fig. 2.8, we note that the straight line used to determine point Y also represents the unloading curve after a maximum stress σY has been reached. While the material does not behave truly elastically, the resulting plastic strain is as small as the selected offset. If, after being loaded and unloaded (Fig. 2.14), the test specimen is loaded again, the new loading curve will closely follow the earlier unloading curve until it almost reaches point C. 35 Lecture 2 ADU 36 MEC 302 2.6 ELASTIC VERSUS PLASTIC BEHAVIOR OF A MATERIAL It will then bend to the right and connect with the curved portion of the original stress-strain diagram. We note that the straight-line portion of the new loading curve is longer than the corresponding portion of the initial one. Thus, the proportional limit and the elastic limit have increased as a result of the strain-hardening that occurred during the earlier loading of the specimen. However, since the point of rupture R remains unchanged, the ductility of the specimen, which should now be measured from point D, has decreased. We assume that the material is mild steel, for which the yield strength is the same in tension and in compression. 36 Lecture 2 MEC 302 ADU 2.6 ELASTIC VERSUS PLASTIC BEHAVIOR OF A MATERIAL 37 Lecture 2 ADU 38 MEC 302 2.6 ELASTIC VERSUS PLASTIC BEHAVIOR OF A MATERIAL The initial load is tensile and is applied until point C has been reached on the stress-strain diagram (Fig. 2.15). After unloading (point D), a compressive load is applied, causing the material to reach point H, where the stress change is equal to 2σY. We note that portion DH of the stress-strain diagram is curved and does not show any clearly defined yield point. This is referred to as the Bauschinger effect. As the compressive load is maintained, the material yields along line HJ. If the load is removed after point J has been reached, the stress returns to zero along line JK, and we note that the slope of JK is equal to the modulus of elasticity E. 38 Lecture 2 ADU 39 MEC 302 2.6 ELASTIC VERSUS PLASTIC BEHAVIOR OF A MATERIAL The resulting permanent set AK may be positive, negative, or zero, depending upon the lengths of the segments BC and HJ. If a tensile load is applied again to the test specimen, the portion of the stress-strain diagram beginning at K (dashed line) will curve up and to the right until the yield stress σY has been reached. If the initial loading is large enough to cause strainhardening of the material (point C’), unloading takes place along line C’D’. As the reverse load is applied, the stress becomes compressive, reaching its maximum value at H’ and maintaining it as the material yields along line H’J’. We note that while the maximum value of the compressive stress is less than σY, the total change in stress between C’ and H’ is still equal to 2σY 39 Lecture 2 ADU 40 MEC 302 2.6 ELASTIC VERSUS PLASTIC BEHAVIOR OF A MATERIAL If point K or K’ coincides with the origin A of the diagram, the permanent set is equal to zero, and the specimen may appear to have returned to its original condition. However, internal changes will have taken place and, while the same loading sequence may be repeated, the specimen will rupture without any warning after relatively few repetitions. This indicates that the excessive plastic deformations to which the specimen was subjected have caused a radical change in the characteristics of the material. Reverse loadings into the plastic range, therefore, are seldom allowed, and only under carefully controlled conditions. Such situations occur in the straightening of damaged material and in the final alignment of a structure or machine. 40 Lecture 2 MEC 302 ADU 2.6 ELASTIC VERSUS PLASTIC BEHAVIOR OF A MATERIAL 41 Lecture 2 ADU 42 MEC 302 2.7 REPEATED LOADINGS; FATIGUE As we know that if the maximum stress in the specimen does not exceed the elastic limit of the material, the specimen returns to its initial condition when the load is removed. You might conclude that a given loading may be repeated many times, provided that the stresses remain in the elastic range. Such a conclusion is correct for loadings repeated a few dozen or even a few hundred times. However, as you will see, it is not correct when loadings are repeated thousands or millions of times. In such cases, rupture will occur at a stress much lower than the static breaking strength σB; this phenomenon is known as fatigue. Hence a fatigue failure is of a brittle nature, even for materials that are normally ductile. 42 Lecture 2 ADU 43 MEC 302 2.7 REPEATED LOADINGS; FATIGUE Fatigue must be considered in the design of all structural and machine components that are subjected to repeated or to fluctuating loads. The number of loading cycles that may be expected during the useful life of a component varies greatly. For example, a beam supporting an industrial crane may be loaded as many as two million times in 25 years (about 300 loadings per working day) An automobile crankshaft will be loaded about half a billion times if the automobile is driven 200,000 miles, and an individual turbine blade may be loaded several hundred billion times during its lifetime. 43 Lecture 2 ADU 44 MEC 302 2.7 REPEATED LOADINGS; FATIGUE The number of loading cycles required to cause the failure of a specimen through repeated successive loadings and reverse loadings may be determined experimentally for any given maximum stress level. If a series of tests is conducted, using different maximum stress levels, the resulting data may be plotted as a σ-n (S-N) curve. For each test, the maximum stress σ is plotted as an ordinate and the number of cycles n as an abscissa; because of the large number of cycles required for rupture, the cycles n are plotted on a logarithmic scale. A typical σ-n curve for steel is shown in Fig. 2.16. We note that, if the applied maximum stress is high, relatively few cycles are required to cause rupture. 44 Lecture 2 ADU 45 MEC 302 2.7 REPEATED LOADINGS; FATIGUE As the magnitude of the maximum stress is reduced, the number of cycles required to cause rupture increases, until a stress, known as the endurance limit, is reached. The endurance limit is the stress for which failure does not occur, even for an indefinitely large number of loading cycles. For a low-carbon steel, such as structural steel, the endurance limit is about one-half of the ultimate strength of the steel. For nonferrous metals, such as aluminum and copper, a typical σ-n curve (Fig. 2.16) shows that the stress at failure continues to decrease as the number of loading cycles is increased. For such metals, one defines the fatigue limit as the stress corresponding to failure after a specified number of loading cycles, such as 500 million. 45 Lecture 2 MEC 302 ADU 2.7 REPEATED LOADINGS; FATIGUE 46 Lecture 2 ADU MEC 302 47 Lecture 2 MEC 302 48 ADU Variable Cross-sectional Area 48 Lecture 2 ADU Example 2.01 SOLUTION: Divide the rod into components at the load application points. Apply a free-body analysis on each component to determine the internal force MEC 302 E 200GPa Evaluate the total of the component deflections. Determine the deformation of the steel rod shown under the given loads. 3- 49 Lecture 2 ADU Example 2.01 SOLUTION: Divide the rod into three components: Apply free-body analysis to each component to determine internal forces, P1 240 kN P2 60 kN P3 120 kN MEC 302 Evaluate total deflection, L1 L2 300 mm. L3 400 mm. A1 A2 580 mm 2 A3 190 mm 2 1.729 mm 3- 50 Lecture 2 ADU 51 MEC 302 Deformation is Measured by the Relative Displacement The deformation of the rod is measured by the relative displacement of one end of the rod with respect to the other Let us consider, for instance, the assembly shown in Fig. 2.20a, which consists of three elastic bars of length L connected by a rigid pin at A. If a load P is applied at B (Fig. 2.20b), each of the three bars will deform. Since the bars AC and AC’ are attached to fixed supports at C and C’, their common deformation is measured by the displacement δA of point A. On the other hand, since both ends of bar AB move, the deformation of AB is measured by the difference between the displacements δA and δB of points A and B, i.e., by the relative displacement of B with respect to A. 51 Lecture 2 Denoting this relative displacement by δB/A, we write MEC 302 52 ADU Deformation is Measured by the Relative Displacement 52 Lecture 2 ADU MEC 302 53 Lecture 2 ADU MEC 302 54 Lecture 2 ADU MEC 302 55 Lecture 2 The rigid castings A and B are connected by two 18 mm diameter steel bolts CD and GH and are in contact with the ends of a 38 mm diameter aluminum rod EF. Each bolt is single-threaded with a pitch of 2.5 mm, and after being snugly fitted, the nuts at D and H are both tightened one-quarter of a turn. Knowing that E is 200 GPa for steel and 70 GPa for aluminum, determine the normal stress in the rod. 56 ADU Sample Problem 2.2 MEC 302 450 mm 300 mm 56 Lecture 2 ADU MEC 302 57 Sample Problem 2.2 57 Lecture 2 ADU MEC 302 58 Sample Problem 2.2 58 Lecture 2